127RMZ – Materials and Geoenvironment, Vol. 57, No. 1, pp. 127–142, 2010
Differential thermal analysis (DTA) and differential scanning calorimetry (DSC) as a method of material investigation
Diferenčna termična analiza (DTA) in diferenčna vrstična kalorimetrija (DSC) kot metoda za raziskavo materialov
GreGa klančnik1, *, joŽeF Medved1, PriMoŽ Mrvar1
1University of Ljubljana, Faculty of natural science and engineering, Department of materials and metallurgy, Aškerčeva 12, SI-1000 Ljubljana, Slovenia
*Corresponding author. E-mail: firstname.lastname@example.org
Received: August 17, 2009 Accepted: December 8, 2009
Abstract: Thermal analysis is used to establish thermodynamic properties which are essential for understanding the behavior of material under different heating and cooling rates, under inert, reduction or oxida- tion atmosphere or under different gas pressures. Thermal analysis comprises a group of techniques in which a physical property of a substance is measured to a controlled temperature program. In this paper only two methods are presented: differential thermal analy- sis (DTA) and differential scanning calorimetry (DSC). The results given from the DTA or DSC curves depend on the preparation of the material, and on the instrument sensitivity. The sensitivity is in close relation to the apparatuses design. Several types of DTA and DSC apparatuses are described as well as the use. New types of DSC devices are being developed which will have the capability of high heating / cooling rates and with shorter response time.
Izvleček: Termična analiza podaja termodinamske lastnosti materiala, ki so pomembne za razumevanje vedenja materiala pri različnih segrevalnih in ohlajevalnih hitrostih, bodisi v inertni, redukcijski ali oksidacijski atmosferi ali pri različnih tlakih. Termična analiza združuje skupino tehnik, kjer je preiskovan vzorec izpostavljen kon- troliranemu temperaturnemu programu. V tem članku sta predstav- ljeni le dve metodi: diferenčna termična analiza (DTA) in simultana termična analiza (STA). Rezultati so bolj ali manj odvisni od priprave
128 klančnik, G., Medved, j., Mrvar, P.
RMZ-M&G 2010, 57
vzorca in nazadnje tudi od občutljivosti naprave. Občutljivost mer- jenja je v ozki povezavi s konstrukcijo naprave. V tem članku so opisani različni tipi DTA- in DSC-naprav ter možna uporaba le-teh. Novi tipi DSC-naprav se razvijajo v smeri visokih hitrostih seg- revanja in ohlajevanja z majhnimi odzivnimi časi.
Key words: DTA, DSC, thermal analysis Ključne besede: DTA, DSC, termična analiza
Thermal analysis (TA) Thermal analysis comprises a group of techniques where the properties of material are studied as they change with temperature. To determine the thermo-physical properties several methods are commonly used: differ- ential thermal analysis (DTA), dif- ferential scanning calorimetry (DSC), thermogravimetric analysis (TGA), dilatometry (DIL), evolved gas anal- ysis (EGA), dynamic mechanical analysis (DMA), dielectric analyse (DEA) etc. In metallurgy, material science, pharmacy and food indus- try the main application of the DTA and DSC is used for studying phase transition under different atmospheric influences, temperatures and heating / cooling rates. Common laboratory equipment has a combination of two thermal analysis techniques. Most common is the simultaneous thermal analysis (STA) apparatus as the com- bination of thermogravimetric analy- sis (TGA) and differential thermal analysis (DSC).
Definitions of DTA and STA methods The two methods (DTA and DSC) are defined as followed:
Differential thermal analysis (DTA): Thermal analysis using a reference. The sample and the reference material (sample) are heated in one furnace. The difference of the sample temperature and the reference material temperature is recorded during programmed heat- ing and cooling cycles.
Differential Scanning Calorimetry (DSC): Differential Scanning Calor- imetry (DSC) measures the change of the difference in the heat flow rate to the material (sample) and to a reference material while they are subjected to a controlled temperature program.
Like differential thermal analysis (DTA), differential scanning (DSC) is also an alternative technique for deter- mining the temperatures of the phase transitions like melting point, solidifi- cation onset, re-crystallization onset, evaporation temperature etc. With dif- ferential thermal analysis DTA, which
129Differential thermal analysis (DTA) and differential scanning calorimetry (DSC) ...
RMZ-M&G 2010, 57
is an older technique than differential scanning calorimetry, the result is a DTA curve (Figure 1b). DTA curve is a curve of temperature difference be- tween the sample material and the ref- erence material versus temperature or time. The result of DSC is a curve of heat flux versus time or temperature and is therefore used also for deter- mination of the enthalpy, specific heat (cp) etc.
 Heat flow rate signal (DSC signal) is internally calculated from the temperature difference between the sample material and the reference material. The important difference be- tween DSC and DTA equipment is that the latter is mostly used for the quali- tative measurements and it is more ro- bust because of less sensitive materials used for sample holders, heat conduc- tion path etc. The sample holder in the DTA apparatus is much cheaper than
the sample holder in the DSC apparatus and is recommended for the investiga- tion of materials with an unknown rela- tion to contamination between the cru- cible and the sample holders. Sample holders are commonly made of Al2O3 with integrated thermocouples. In the case of DSC the technique is more sen- sitive and allows several modifications which make it possible to measure the thermal conductivity, evolved gas anal- ysis, thermogravimetry and activation energy for the grain growth, precipita- tion, etc. Sampler holders are common- ly made of platinum.
It is typical for the DTA that the sample and the reference material are under iden- tical temperature regime. This is not true in the case of the DSC method. In this case the method with two furnaces can also be used (Power compensation DSC).
Figure 1. DTA heating curve for pure Ag (10 K/min): the sample and the reference temperature (a) and DTA signal as dependence of time and tem- perature (b)
130 klančnik, G., Medved, j., Mrvar, P.
RMZ-M&G 2010, 57
Where: tS,C, tW,C, tT,C – characteristic times for the heat flow between the metal sample and the crucible cup, the furnace wall and the crucible cup, the thermocouple and the crucible cup
hT,CAT,C, hW,CAW,C, hS,CAS,C - products of heat transfer coefficient and areas of heat flow mC, mT – mass of the crucible (C) and the thermocouple (T)
c P CC , - heat capacity (J/K)
dIfferentIal thermal analysIs (dta)
Differential thermal analysis (DTA) was constructed soon after the devel- opment of the thermocouple (1887, Le
T ptS,C = mTC / hT,CAT,C
Two basic types of Differential Scan- ning Calorimetry (DSC) must be dis- tinguished: the heat flux DSC and the power compensation DSC. Sometimes a third basic type is also distinguished called the Hyper DSC which is an ap- paratus for rapid solidification based on power compensation DSC. Figure 2 represents both basic types of DSC apparatuses.
The power compensation DSC or PC – DSC has an individual heater for each chamber (figure 2 a). In the case of the heat flux or HF – DSC, both the sample and the reference material are inside the same furnace. The HF - DSC is also known as a type of Boersma DTA. The PC – DSC is more effective because the time constants (characteristic response time) are shorter. The characteristics of each device can be described with three characteristic times:
Figure 2. Shematic layout of the DSC apparatus: PC-DSC (a) and quanti- tative (Boersma) DTA or HF-DSC (b)
tS,C = mCC / hS,CAS,C C p
C ptW,C = mCC
131Differential thermal analysis (DTA) and differential scanning calorimetry (DSC) ...
RMZ-M&G 2010, 57
Chatelier). It was made for the exami- nation of different materials. Most of the research efforts were made on clay and carbonate materials. The limitation in the DTA apparatuses is its sensitiv- ity. This is shown by the next mineral called limonite. The difference in the DTA and DSC heating curves are rep- resented in figure 3.
In figure 3 a at least three separate de- compositions were determined by the DSC and TG curve. The DTA curve showed only one because the quantity of the released heat was too small to be detected.
Nevertheless, the DTA curves can record the transformations where the heat is either absorbed or released (de- hydration, decarbonation, burning of materials, ordering etc.). DTA is help- ful for better understanding of given results by x-ray diffraction, chemical analysis and microscopy.
The most important advantages of the DTA are its simplicity and a possibility to create different experimental condi- tions (high pressure or vacuum).
DTA can also be used for quantita- tive measurements (enthalpy meas- urements). The DTA has advantages over DSC because it allows simultane- ous recor